Unusual High Thermal Stablility of a 2D →3D Polycatenated Fe(II) Metal‒Organic Framework Showing Guest-Dependent Spin-Crossover Behavior and High Spin-Transition Temperature
Zhang, Xiu-Tang; Sun, Di; Li, Bao; Fan, Li-Ming; Li, Bin; Wei, Pei-Hai; Crystal Growth & Design 12 (2012) 3845–; doi:10.1021/cg3007876

data_4506569
_publ_section_title
;
 Unusual High Thermal Stablility of a 2D \\rightarrow 3D Polycatenated
 Fe(II) Metal--Organic Framework Showing Guest-Dependent Spin-Crossover
 Behavior and High Spin-Transition Temperature
;
_journal_issue                   8
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              3845
_journal_paper_doi               10.1021/cg3007876
_journal_volume                  12
_journal_year                    2012
_chemical_formula_moiety         'C36 H24 Fe N10, H2 O'
_chemical_formula_sum            'C36 H26 Fe N10 O'
_chemical_formula_weight         670.52
_chemical_name_systematic
; 
 ? 
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           60
_space_group_name_Hall           '-P 2n 2ab'
_space_group_name_H-M_alt        'P b c n'
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   19.533(2)
_cell_length_b                   8.3503(9)
_cell_length_c                   19.621(2)
_cell_measurement_reflns_used    1033
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      43.990
_cell_measurement_theta_min      5.306
_cell_volume                     3200.3(6)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0422
_diffrn_reflns_av_sigmaI/netI    0.0304
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            15095
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.08
_exptl_absorpt_coefficient_mu    0.519
_exptl_absorpt_correction_T_max  0.9597
_exptl_absorpt_correction_T_min  0.9404
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.392
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1384
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.877
_refine_diff_density_min         -1.291
_refine_diff_density_rms         0.075
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.082
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         2808
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.082
_refine_ls_R_factor_all          0.0671
_refine_ls_R_factor_gt           0.0548
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0842P)^2^+2.7957P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1468
_refine_ls_wR_factor_ref         0.1572
_reflns_number_gt                2210
_reflns_number_total             2808
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg3007876_si_002.cif
_cod_data_source_block           p
_cod_database_code               4506569